Shear Bond Strength of the Repair Composite Resin to Zirconia Ceramic by Different Surface Treatments
Journal of Lasers in Medical Sciences,
Vol. 5 No. 4 (2014),
24 September 2014
Introduction: The purpose of this study is the evaluation of the amount of surface roughness (Ra) of Zirconia Ceramic following different surface treatments as well as the assessment of its shear bond strength to composite resin.
Methods: 40 sintered zirconia ceramic block samples were randomly divided in 4 groups of 10 and underwent the following surface treatments:
a) Control group without treatment
b) Air abrasion with Al2O3 particles (50um)
c) Er:YAG laser with 2W power for 10s
d) Nd:YAG laser with 1.5W power for 2min
Then the mean surface roughness (Ra) was evaluated by profilometer. In the next step, Alloy primer was used on a section of 9mm2 on the samples following the manufacturer’s instructions. After that Clearfil AP-X composite resin in cylinder shape with an internal diameter and height of 3mm were cured on the sections mentioned. At the end, all samples were tested to assess the shear bond strength by the Universal Testing Machine at a speed of 0.5mm/min until fracture occurred. The mean shear bond strengths were calculated and statistically analyzed by One Way ANOVA.
Results: ANOVA analysis showed that roughness (Ra) was significantly different between the groups (P≤0.05). Ra was higher in the Nd:YAG group compared to the other groups (P≤0.05). The lower Ra was related to the control group. Air abrasion group showed highest amounts of shear bond strength and Nd:YAG laser group demonstrated lower amounts of shear bond strength (P≤0.05).
Conclusion: Various surface treatments are differently effective on bond strength. Air abrasion is the most effective method to condition zirconia ceramic surfaces.
- zirconia ceramic
How to Cite
Kim KB, Bae HE , Shim JS, Lee KW. The influence of ceramic surface treatments on the tensile bond strength of composite resin to all-ceramic coping materials . J Prosthet Dent 2005;94:357-62.
Akyil MS, Uzun IH, Bayindir F. Bond Strength of Resin Cement to Yttrium-Stabilized Tetragonal Zirconia Ceramic Treated with Air Abrasion, Silica Coating, and Laser Irradiation. Photomed Laser Surg 2010 ;28(6) : 801–8.
Alaa Hussein Aref Sabrah . The Effect Of Full-Contour Y-Tzp Ceramic Surface Roughness On The Wear Of Bovine Enamel And Synthetic Hydroxyapatite: An In-Vitro Study . Thesis 2011.
Fischer J, Grohmann P, Stawarczyk B. Effect of Zirconia Surface Treatments on the Shear Strength of Zirconia/Veneering Ceramic Composites . Dent Mater J 2008; 27(3): 448－54.
Güler AU, Yilmaz F, Yenisey M, Güler E, Ural C . Effect of acid etching time and a self-etching adhesive on the shear bond strength of composite resin to porcelain. J Adhes Dent 2006;8(1):21-5.
Goia TS, Pereira Leite FP, Valandro LF, Özcan M, Bottino MA . Repair Bond Strength of a Resin Composite to Alumina-Reinforced Feldspathic Ceramic. Int J Prosthodont 2006;19:400–2.
Özcan M, Valandro LF, Amaral R, Leite F, Bottino MA. Bond strength durability of a resin composite on a reinforced ceramic using various repair systems. Dent Mater 2009;25: 1477–83.
Della Bona A, Borba M , Benetti P, Cecchetti D. Effect of surface treatments on the bond strength of a zirconia-reinforced ceramic to composite resin. Braz Oral Res 2007;21(1):10-5.
Bottino MA, Valandro LF, Scotti R, Buso L. Effect of surface treatments on the resin bond to zirconium-based ceramic. Int J Prosthodont. 2005;18(1):60-5.
Piascik JR, Swift EJ, Thompson JY, Grego S, Stoner BR. Surface modification for enhanced silanation of zirconia ceramics. Dent Mater. 2009;25(9):1116-21. doi: 10.1016/j.dental.2009.03.008. Epub 2009 Apr 18.
Kussano CM, Bonfante G, Batista JG, Pinto JH. Evaluation of Shear Bond Strength of Composite to Porcelain According to Surface Treatment . Braz Dent J 2003; 14(2): 132-5.
Foxton RM, Cavalcanti AN, Nakajima M, Pilecki P, Sherriff M, Melo L, et al . Durability of resin cement bond to aluminium oxide and zirconia ceramics after air abrasion and laser treatment . J Prosthodont 2011;20:84-92.
Aydogan Ayaz, Fatih Mehmet Korkmaz, Kıvanç Utku Ulusoy, Yildirim Hakan Bagis. How will surface treatments affect the translucency of porcelain laminate veneers? J Adv Prosthodont. 2014 February; 6(1): 8–13. Published online 2014 February 14. doi: 10.4047/jap.2014.6.1.8
Cavalcanti A, Pilecki P, Foxton RM, Watson TF, Oliveira MT, Gianinni M, et al. Evaluation of the Surface Roughness and Morphologic Features of Y-TZP Ceramics after Different Surface Treatments. Photomed Laser Surg 2009;27:473-9.
Tsuo Y, Yoshida K, Atsuta M. Effects of Alumina-blasting and Adhesive Primers on Bonding between Resin Luting Agent and Zirconia Ceramics. Dent Mater J 2006; 25(4)：669－74.
Prabu PS , Prabu N. Composite as a Ceramic Repair Material – An Invitro Study. J Ind Aca Dent Spec 2010 ; 1(4): 27-32.
Kim BK, Bae HE, Shim JS, Lee KW. The influence of ceramic surface treatments on the tensile bond strength of composite resin to all-ceramic coping materials. J Prosthet Dent 2005;94:357-62.
Yang B, Barloi A, Kern M. Influence of air-abrasion on zirconia ceramic bonding using an adhesive composite resin. Dent Mater 2010; 26: 44–50.
Kern M, Barloi A, Yang B. Surface Conditioning Influences Zirconia Ceramic Bonding. J Dent Res 2009;88(9):817-22.
Matinlinna JP, Lassila LV. Enhanced resin-composite bonding to zirconia framework after pretreatment with selected silane monomers . Dent Mater 2011;27(3) : 273–80.
Kim MJ, Kim YK, Kim KH, Kwon TY. Shear bond strengths of various luting cements to zirconia ceramic: Surface chemical aspects. J Dent 2011; 39(11):795–803.
Subaşı MG, İnan Ö. Evaluation of the topographical surface changes and roughness of zirconia after different surface treatments . Lasers Med Sci 2012;27(4):735-42. DOI 10.1007/s10103-011-0965-3
Akin H, Tugut F, Akin GE, Guney U, Mu-taf B. Effect of Er:YAG laser application on the shear bond strength and microleakage be-tween resin cements and Y-TZP ceramics. Laser med sci. 2012; 27: 333-8
- Abstract Viewed: 275 times
- PDF Downloaded: 142 times